Strain rate effect on tensile behavior of the helical multi-shell gold nanowires
Page content transcription ( If your browser does not render page correctly, please read the page content below )
Materials Chemistry and Physics 100 (2006) 48–53 Strain rate effect on tensile behavior of the helical multi-shell gold nanowires Shin-Pon Ju a , Wen-Jay Lee a , Jenn-Sen Lin b,∗ , Ming-Liang Liao c a Department of Mechanical and Electro-Mechanical Engineering; Center for Nanoscience and Technology, National Sun-Yat-Sen University, Kaohsiung, Taiwan 804, Republic of China b Department of Mechanical Engineering, National United University, Miao-Li, Taiwan 360, Republic of China c Department of Aircraft Engineering, Air Force Institute of Technology, Kaohsiung, Taiwan 820, Republic of China Received 17 April 2005; received in revised form 4 November 2005; accepted 5 December 2005 Abstract A molecular dynamics simulation of the helical multi-shell (HMS) gold nanowires for tensile behavior has been carried out at 4 K temperature. HMS nanowires, not like bulk face centered cubic (FCC) structure, have a multi-shell helical structure. This work compares mechanical properties and deformation behaviors of the 7-1, 11-4 and 14-7-1 multi-shell helical structure under different strain rates. The results reveal that the different strain rate influence the maximum stress, Young’s modulus and deformation behaviors. The Young’s modulus and maximum stress of HMS nanowires are function of the ratio of numbers of surface atoms to the total number of atoms, but tubular 11-4 HMS nanowire is an exception. For different strain rate, many different deformation behaviors are appear which include sliding, multi-sliding, phase transformative, twisting, necking and brittle deformations before breaking. © 2005 Elsevier B.V. All rights reserved. Keywords: Molecular dynamics; Tight-binding potential; Nanowire; Helical muti-shell structures; Tensile test 1. Introduction vary from 0.6 to 1.2 nm. The thinnest gold nanowire exhibits a 7-1 shell structure with a diameter of about 0.6 nm, and two One-dimensional nanowires have attracted great interest in other nanowires are 11-4 and 14-7-1. Therefore, the structures recent years because they have broad applications in differ- of the HMS gold nanowires are different from those of the face ent areas, such as in nano-mechanical and nano-electronic centered cubic (FCC) crystalline bulk, influencing mechanical devices. Metallic nanowires with well-defined structures of sev- properties and electrical transportation. eral nanometers in size have been fabricated by using various Some fundamental studies have investigated the physi- methods [1–12]. As the scale is reduced to nanometers, the cal properties of metallic nanowires, by simulating molecular surface, small size and quantum effect dramatically changes dynamics [13–27]. For example, metal nanotubes or nanowires the physical and transport phenomena. Gold nanowire becomes have been melted [13–15], and the interior melting tempera- quantization of electronic conductance as their diameter is ture in ultrathin nanowires has been found to be lower than reduced to 2 nm . In recent works, helical multi-shell (HMS) that at the surface. Ultrathin Cu nanotubes collapsed into the structures have been observed in gold nanowires [1,2] by trans- empty core at low temperature and this is the main mecha- mission electron microscopy (TEM). These gold nanowires con- nism for the transformation from ultrathin nanotube to nanowire sist of coaxial tubes with n, n and n helical atom rows, where . The mechanical behavior of the copper nanowires in n, n and n denote the number of atoms in the outer, middle and a tensile test has been studied [17,18]. Unusual pentagonal inner shells, respectively; moreover, tubes with an odd number structure in Cu nanowires was found mechanical stretching of atoms present a helical structure, whereas those with an even [19,20]. The strain rate effect induced by amorphizations of number of atoms do not, The HMS gold nanowires diameters Ni nanowires has also been investigated by using molecular dynamics simulation . Moreover, the formation of single- atom chains consisting of metal atoms was observed and ∗ Corresponding author. Tel.: +886 373 81321; fax: +886 373 81333. studied by experiments and molecular dynamics simulations E-mail address: firstname.lastname@example.org (J.-S. Lin). [22–27]. 0254-0584/$ – see front matter © 2005 Elsevier B.V. All rights reserved. doi:10.1016/j.matchemphys.2005.12.005
S.-P. Ju et al. / Materials Chemistry and Physics 100 (2006) 48–53 49 Table 1 Parameter used in tight-binding potential Au A (eV) 0.2061 ξ (eV) 1.790 p 10.229 q 4.036 r0 (Å) 2.885 interaction force on atom i is given by: ∂Ei ∂Ej Fi = − + (2) ∂rij ∂rij j=i Fig. 1. Schematic diagram for constructing multi-shell structure nanowires. Table 1 lists the parameters of the tight-binding potential associated with Au in the current simulation . The loading state in the molecular dynamics simulation for This work applies molecular dynamics simulation to study the tensile test is as follows; the loading is applied along the axis, the mechanical behavior and deformation behaviors of gold and top and bottom layers are set as fixed layers; the others are nanowires with three types of multi-shell helical structures, 7-1, set as thermal controlled layers. The following scaling method 11-4 and 14-7-1 structures, under various strain rates. In this is adopted to ensure that the temperature of the system remains study, all simulations are set at a temperature of 4 K. constant during simulation : TD 2. Molecular dynamics simulation vi = vi new (3) TA Ultrathin gold nanowires with a multi-shell helical structure where vnew i is the velocity of particle i after correction. TD and have been recently fabricated . In this simulation, the multi- TA are the desired and actual temperatures of the system, respec- shell helical structures are constructed and originating from tively. This scaling method is applied during the simulation for Au(1 1 1) plane, being rolled up with certain helical angle. Fig. 1 a specific equilibrium temperature. presents three types of multi-shell structure, i.e., 7-1, 11-4 and The stress in the atomistic simulation σ mn on m-plane and 14-7-1. For 7-1 and 14-7-1, those multi-shell configurations have n-direction is calculated as: a single central strand of gold atoms and a tube structure formed ⎡ ⎤ from helices of atoms coiled around the axis of the tube; for 1 ⎣ mi vm v n 1 ∂φ(rij ) rijm rijn σmn = i i − ⎦ (4) 11-4, it could be presumed as a cannular type of nanowire. NS Vi 2Vi ∂rij rij The many-body tight-binding potential is employed to simu- i j late the interatomic force between the gold atoms [28,29]. The where mi is the mass of atom I, Vi the volume assigned around to main difference between the many-body potential model and atom I, NS the number of particles contained in region S, where a pairwise potential model is that the interaction between two S is defined as the region of atomic interaction, rij the distance atoms is considered in the former case to depend not only on two between atoms i and j, and rijm and rijn are the two components of atoms, but also upon their local environment. The tight-binding the vector from atom i to j. The first term of the right hand side potential model commences by summing the band energy, which of Eq. (4) represents the kinetic effect associated with atomic is characterized by the second moment of the d-band density of motion, and will be affected by temperature. The second term state, and a pairwise potential energy of the Born–Mayer type. is related to the interactive forces and the distance between the The cohesive energy is thus expressed as follows: atoms. ⎧ ⎡ ⎤1/2 ⎫ n ⎪⎨ ⎪ ⎬ ⎣ rij ⎦ + rij Ec = − ξ exp −2q 2 −1 A exp −p −1 (1) ⎪ r0 r0 ⎪ i=1 ⎩ j j ⎭ The normal strain in the axial direction ε is calculated as: where ξ is an effective hopping integral, rij the distance between atom i and j, and r0 is the first-neighbor distance. The parameters lz(t) − lz(0) A, p, q and ξ are determined by the experimental data concern- ε= (5) lz(0) ing cohesive energy, lattice parameter, bulk modulus and shear elastic constants C44 and C = 1/2(C11 − C12 ), respectively. Fur- where lz(t) is the average length in the axial direction and lz(0) thermore, the force as negative gradient of cohesive energy, the is the average initial length. Thus, the stress–strain relationship
50 S.-P. Ju et al. / Materials Chemistry and Physics 100 (2006) 48–53 of the ultrathin gold nanowires can be obtain using Eqs. (4) and show stress–strain relationship and deformed morphologies of (5). 7-1 MHS nanowires for various strain rates. At a lower strain The Verlet algorithm  is employed to calculate the trajec- rate, 0.003% ps−1 , the stress–strain curve shows a zigzag of tories of the atoms and in the tensile test, the loading is applied increase–decrease in stress as the strain is increased. The max- to the Au nanowires after relaxation for 50 ps. imum stress is located at first yielding point, σ 33 = 7.0 GPa and ε = 0.07, and the deformed zone are near to middle region. 3. Results and discussion Increasing the strain rate of the tensile test, the stress–strain curves become smooth. The yielding stress increases first then This study addresses tensile tests of HMS gold nanowires decreases for large strain rate. When the strain rate is very high, with 7-1, 11-4 and 14-7-1 structures. The engineering stress there is no obviously yielding behavior in stress–strain curve. and strain relationships and the morphologies of the deforma- Snapshots of some critical deformed behavior after yielding are tion for different strain rates are shown in Figs. 2–5. The results shown in Fig. 3(a)–(g). Fig. 3(a)–(d) show the deformed process reveal that the stress–strain relationships and deformed mor- at strain rate 0.003% ps−1 , (e) and (f) are at 0.833% ps−1 and phologies are strongly affected by strain rate. Figs. 2(a) and 3 (g) is at 3.333% ps−1 . For the quite small strain rate, a zigzag Fig. 2. Stress–strain relationships for (a) 7-1, (b) 11-4 and (c) 14-7-1 structure under tensile test.
S.-P. Ju et al. / Materials Chemistry and Physics 100 (2006) 48–53 51 Fig. 3. Morphology of the deformed 7-1 nanowire in different strain at various strain rate of (a)–(d) 0.003% ps−1 ; (e)–(f) 0.833% ps−1 ; (g) 3.333% ps−1 . The strain of all snapshots are (a) ε = 0.122; (b) ε = 0.204; (c) ε = 0.27; (d) ε = 0.451; (e) ε = 0.104; (f) ε = 0.242; (g) ε = 0.152, respectively. Fig. 4. Morphology of the deformed 11-4 nanowire in different strain at various strain rate of (a)–(c) 0.003% ps−1 ; (d)–(e) 0.833% ps−1 ; (f) 3.333% ps−1 . We can see in perspective (a) of the right hand side, the inner shell (black sphere) neck before the out shell (gray sphere) produces after first yielding. The strain of all snapshots are (a) ε = 0.049; (b) ε = 0.051; (c) ε = 0.090; (d) ε = 0.166; (e) ε = 0.299; (f) ε = 0.14, respectively. stress–strain curve implies successive yielding process. From stain rate of 0.833% ps−1 , the maximum stress, σ 33 = 7.2 GPa, Fig. 3(a), the atomic configuration of cross-section is trans- is higher than that of 0.333% ps−1 , and the stress–strain curve formed from that of the 7-1 structure to that of 6-1 structure is more smooth. At this strain rate, the 6-1 structure are formed after yielding. The 6-1 structure suffuses the nanowire gradu- near end of wire after yielding and then necking deformations ally as the strain is increased to 0.13, and the stress raises to near occur at both end side of the wires, as shown in Fig. 3(e) and (f). σ 33 = 5 GPa. Basically, the helical angle between the two areas Moreover, at very high strain rate, 3.333% ps−1 , the maximum apart from the sliding zone remains. Continuing to increase the stress is lower than that at low strain rate. From the stress–strain strain, the 7-1 nanowire is necked and the atomic configura- curve, there is no obviously yielding point at high strain rate. tion of cross-section changes. Fig. 3(b)–(d) show the snapshots Due to very high strain rate, the kinetic energy interaction among which the cross section of the 7-1 nanowire neck to a width of the atoms in the deformed zones has not enough time to trans- four, two and one atom chains at different strains, respectively. fer to others. The brittle type of deformation at two end zones is The dynamics evolution of this quadruple strand, double strand formed and others retain the original 7-1 structure such as shown and single strand can been experimentally observed . For the in Fig. 3(g). Fig. 5. Morphology of the deformed 14-7-1 nanowire in different strain at various strain rate of (a)–(d) 0.003% ps−1 ; (e)–(f) 0.833% ps−1 ; (g) 3.333% ps−1 . The strain of all snapshots are (a) ε = 0.074; (b) ε = 0.106; (c) ε = 0.246; (d) ε = 0.115; (e) ε = 0.250; (f) ε = 0.655; (g) ε = 0.096, respectively.
52 S.-P. Ju et al. / Materials Chemistry and Physics 100 (2006) 48–53 Figs. 2(b) and 4 presents stress–strain relationship and deformed morphologies of 11-4 MHS nanowires for various strain rates. For small strain rate, 0.003% ps−1 , the maximum stress is near to σ 33 = 4 GPa at strain 0.047. Comparing to the 7-1 nanowire, the maximum stress is much lower. From the morphol- ogy of deformation at low strain rate as shown in Fig. 4(a)–(c), it can be found that the tubular wires are necked in the inner shell just after maximum stress. This behavior is not the same as 7-1 nanowire. This kind of behavior is due to instability of tubu- lar wire under tension. Again, increasing the strain, the wire begins to slide, and the structure reconstruct to a tight struc- ture at strain 0.05, as show in Fig. 4(b). Continuing to increase the strain, the stress is rise again, and the stress is approach to σ 33 = 3.6 GPa at strain 0.09. After strain 0.09, the sliding and necking deformation is observed in Fig. 4(c). Owing to the fact that the 11-4 structure can be treated as a hollow tube, the wire becomes unstable as the side deformation increases. Therefore, the 11-4 structure of a nanotube, because of its tubular structural characteristics, yields more easily than 7-1 and 14-7-1 structure. In Fig. 4(d and e), we show the snapshots of the system at strains for a higher strain rate 0.833% ps−1 , the deformation behaviors is also different from that of thinnest 7-1 structure. The tight Fig. 6. Maximum stress vs. strain rate for HMS nanowires at 4 K. atom of surface structure of 11-4 nanowire is extended to a FCC structure at both end side of the wire as show in Fig. 4(d). More- over, the phase transform cause the 11-4 nanowire to have a 1 nanowires are almost unchanged over a large range of strain higher maximum stress. The new structure allows the system to rate, and the values of maximum stress are near to 7, 4 and support a higher stress. Increasing the strain, the wire necked at 4.8 GPa, respectively. General speaking, the maximum stress is both side, showing in Fig. 4(e), through breaking. At very high function of the ratio of numbers of surface atoms to the total num- strain rate, 3.333% ps−1 , the maximum stress is lower than that ber of atoms, and increases with smaller cross-section [24,31]. at low strain rate. From the stress–strain curve, there is no obvi- However, owing to the 11-4 HMS nanowire can be treat as a ously yielding point at high strain rate just like the 7-1 nanowire. nanotube, which will be easily buckled at inner shell under ten- The brittle type of deformation at two end zones is formed and sion, the strength of 11-4 nanowire is lower comparing to 14-7-1 others retain the original 11-4 structure shown in Fig. 4(f). nanowire. Up to a strain rate of 109 s−1 , the maximum stress have Figs. 2(c) and 5 shows the stress and strain relationships for a slightly increase, because the different deformation behavior the 14-7-1 nanowire at various strain rates. The stress–strain from lower strain rate are occur as previous description. How- relationship of 14-7-1 nanowire is like as that of 7-1 nanowire. ever, the maximum stress decrease after a very high strain rate It could be found that the maximum stress increases as strain of 1010 s−1 , and the brittle deformation are formed at small area rate increasing for low strain rate, however, decreases as strain and others retain the original structures on 7-1, 11-4 and 14- rate increasing for high strain rate. Snapshots of some critical 7-1 nanowires. The stress concentration is observed near the deformed behavior after yielding are shown in Fig. 5(a)–(h). In top and bottom sides, and the interaction among the atoms in Fig. 5(a)–(c), snapshots of the system at several strains for strain the deformed zones has not enough time to transfer to other rate 0.003% ps−1 are shown. The sliding deformation occurs at atoms. In Fig. 6, the engineering stress and engineering strain strain 0.074 after first yielding as shown in Fig. 5(a). Further are adopted. This could not present the true state of the stress increasing the strain to 0.106, the necking deformation causes concentration exactly. the wire pack to a cross section of 10-4 structure as shown in Fig. 7 displays the effect of strain rate on Young’s modulus Fig. 5(b). Finally, the wire is necked to one atom width before at 4 K. In this article, the force approach is adopted to evaluate breaking. At a higher the strain rate 0.833% ps−1 , the defor- the Young’s modulus of the nanowires. The Young’s modulus mation behaviors is different from the other two molded HMS derived from the engineering approach which so call engineer- nanowires. The multi-sliding occurred after yielding as show in ing Young’s modulus, and it can be determined from the results Fig. 5(d). Increasing strain again, the necked deformation hap- of tensile and compressed tests for the strain ε < 2% using linear pen at both end side, and then one atom chain also could be found regression . The Young’s moduli are almost unchanged over before breaking as shown in Fig. 5(e and f). For very high strain a large range of strain rate for 7-1, 11-4 and 14-7-1 HMS struc- rate, 3.333% ps−1 , no more obviously yielding can be found. tures, and the values are 147, 112 and 100 GPa, respectively. The brittle deformation at both end of the wire is also observed The Young’s moduli of HMS nanowires are higher than that of in 14-7-1 nanowire as shown in Fig. 5(g). FCC structure . However, up to a strain rate of 1010 s−1 , Fig. 6 shows the effect of strain rate on maximum stress at the Young’s modulus is decrease as the strain rate is increased, temperature 4 K. The maximum stress of 7-1, 11-4 and 14-7- because the engineering stress is employed.
S.-P. Ju et al. / Materials Chemistry and Physics 100 (2006) 48–53 53 Numbers NSC-92-2212-E-239-003 and NSC-93-2212-E-110- 022. References  Y. Kondo, K. Takayangi, Science 289 (2000) 606.  K. Takayangi, Y. Kondo, H. Ohnishi, JSAP Int. 3 (2001) 3.  Y. Kondo, K. Takayangi, Phys. Rev. Lett. 79 (1997) 3455.  K. Takayangi, Gold Bull. 37 (2004) 138.  V. Rodrigues, D. Ugate, Phys. Rev. B 63 (2001), 073405-1.  M. Barbic, J.J. Mock, D.R. Smith, S. Schultz, J. Appl. Phys. 91 (2002) 9341.  S. Michotte, S.M. Tempfli, L. Piraux, Appl. Phys. Lett. 82 (2003) 4119.  Y. Oshima, H. Koizumi, K. Mouri, H. Hirayama, K. Takayanagi, Phys. Rev. B 65 (2002) 121401.  T.T. Albrecht, J. Schotter, G.A. Kastle, N. Emley, Science 290 (2000) 2126.  T. Sugawara, G.G. Coyle, M.R. Hembree, Scheinfein, Appl. Phys. Lett. 70 (1997) 1043.  R. Sordan, M. Burghard, K. Kern, Appl. Phys. Lett. 79 (2001) 2073.  Z. Tang, N.A. Kotov, M. Giersig, Science 297 (2002) 237.  J. Wang, X. Chen, G. Wang, B. Wang, W. Lu, J. Zhao, Phys. Rev. B 66 (2002) 085408.  G. Bilalbegovic, Solid State Commun. 115 (2000) 73. Fig. 7. Young’s modulus vs. strain rate for HMS nanowires at 4 K.  G. Bilalbegovic, Vacuum 71 (2003) 165.  J.W. Kang, J.J. Seo, H.J. Hwang, J. Phys.: Condens. Matter 14 (2002) 8997. 4. Conclusion  J. Schiotz, K.W. Jacobsen, Science 301 (2003) 1357.  W.J. Chang, T.H. Fang, J. Phys. Chem. Solids 64 (2003) 1279.  J.C. González, V. Rodrigues, J. Bettini, L.G.C. Rego, A.R. Rocha, P.Z. The molecular dynamics simulation is applied to study the Coura, S.O. Dantas, F. Sato, D.S. Galvao, D. Ugarte, Phys. Rev. Lett. 93 stress–strain relationship of the HMS gold nanowires at tem- (2004) 126103. perature 4 K for various tensile velocity. The results show that  J.W. Kang, H.J. Hwang, J. Phys.: Condens. Matter 14 (2002) 2629. the 7-1 structure has the highest maximum stress, and the max-  P.S. Branicio, J.P. Rino, Phys. Rev. B 62 (2000) 16950. imum stress of 7-1 and 14-7-1 structure with a diameter of 0.6  G. Rubio-Bollinger, S.R. Bahn, N. Agrait, K.W. Jacobsen, S. Vieira, Phys. Rev. Lett. 87 (2001) 026101. and 1.0 nm, respectively, are stronger than that of tubular 11-  E.Z. da Silva, A.J.R. da Silva, A. Fazzio, Phys. Rev. Lett. 87 (2001) 256102. 4 structure with a diameter of 0.8 nm. The strain rates affect  S.P. Ju, J.S. Lin, W.J. Lee, Nanotechnology 15 (2004) 1221. Young’s modulus, maximum stress and deformation behaviors.  P.Z. Coura, S.B. Legoas, A.S. Moreira, F. Sato, V. Rodrigues, S.O. Dantas, For various strain rates, the deformation behaviors are different D. Ugarte, D.S. Galvao, Nano Lett. 4 (2004) 1187. on different type HMS nanowires. The HMS nanowires formed  S.W. Hla, K.-F. Braun, V. Iancu, A. Deshpande, Nano Lett. 4 (2004) 1997. a close packing structure after failure at a strain rate lower than  J.S. Lin, S.P. Ju, W.J. Lee, Phys. Rev. B 72 (2005) 85448. 5 × 108 s−1 , two or more deformation zones appear at a higher  V. Rosato, M. Guillope, B. Legrand, Philos. Mag. A 59 (1989) 321. strain rates, and brittle deformation zones are obtained at a very  F. Cleri, V. Rosato, Phys. Rev. B 48 (1993) 22. high strain rates.  J.M. Haile, Molecular Dynamics Simulation, John Wiley & Sons, Canada, 1992.  H. Liang, X. Wang, H. Wu, Y. Wang, Acta Mech. Sin. 34 (2002) Acknowledgement 208.  W.J. Chang, T.H. Fang, J. Phys. Chem. Solids 64 (2003) 1279. The authors would like to thank the National Science Council of the Republic of China for supporting this study, under Grant
Pages you may also like
You can also read
Next part ... Cancel